J. Phys. Chem. B 2001, 105, 7998-8006
Water Adsorption on Activated Carbons: Study of Water Adsorption in Micro- and Mesopores Juan Alcan˜ iz-Monge,*,†,‡ Angel Linares-Solano,† and Brian Rand‡ Departamento de Quı´mica Inorga´ nica, UniVersidad de Alicante, Alicante E-03080, Spain, Department of Materials, UniVersity of Leeds, Leeds LS2 9JT, U.K. ReceiVed: February 21, 2001; In Final Form: June 18, 2001
The mechanism of water adsorption is analyzed in a range of activated carbons differing widely in the relative proportions of narrow and wide micropores, mesopores, and macropores. They also display different degrees of surface functionality. By assuming that the adsorbed phase in micropores is “ice-like”, it is shown that the whole micropore volume is filled with water at a P/P0 of about 0.82, at which point capillary condensation may begin. However, surface complexes control the wetting of the mesopore walls by adsorbed water and can influence the condensation process. Condensation in macropores may also occur at P/P0 values above 0.95. The extent of meso-/macropore filling depends on the surface complexes. The volume filling process is progressive and in micropores is consistent with the theory of volume filling. The adsorption process was analyzed by interpreting the nitrogen isotherms systematically measured on samples of different pore structure with progressively increasing amounts of preadsorbed water up to saturation.
Introduction In many gas treatment processes involving activated carbons (ACs), water vapor is often present and can decrease their performance.1-6 However, the mechanism of water adsorption in carbon materials is complex compared to that of conventional adsorptives (N2, benzene, and CO2).7-15 Two main theories have been invoked to explain the phenomenon of water adsorption in carbon materials. (1) Water adsorption occurs through a capillary condensation mechanism.7,16-22 (2) Water adsorption occurs according to the Dubinin-Serpinsky mechanisms involving clustering around primary adsorption centers.8 The first of these is based on the presence of adsorption hysteresis in the water adsorption isotherms, which is usually associated with the mechanism of capillary condensation.7,16 Juhola17,22 used the Kelvin equation to analyze water adsorption isotherms, suggesting they were suitable alternatives to N2 adsorption for the assessment of pore size distributions. However, both the surface groups and the mineral matter are known to affect the water adsorption isotherm, and so, this method has not received widespread recognition.23 The principal objection has been that the Kelvin equation has no physical basis when applied to water adsorption in micropores because the concepts of meniscus and surface tension lose their macroscopic sense in pores where there is space for only a few adsorbed layers (i.e., 5-7).7 The second mechanism, first postulated by Pierce and Smith24 and further developed by Dubinin and Serpinsky,8,16,25,26 is supported by numerous studies of microporous ACs, which demonstrate a strong influence of surface oxygen complexes on the water adsorption isotherm. In this mechanism, it is assumed that water adsorption occurs through the formation of * Corresponding author. E-mail: [email protected]
† Universidad Alicante. ‡ Leeds University.
clusters of chemisorbed water at active sites that are present on the carbon surface (surface groups), followed by the growth and coalescence of these clusters.8,26 Thus, the surface density and character of these groups controls the relative pressures at which water adsorption starts. Recently, computer simulation studies,27,28 have also indicated that the adsorption of water occurs via the formation of three-dimensional clusters on oxygenated sites, again emphasizing the predominant role that the surface groups have on the water adsorption mechanism. In situ studies of water adsorption using X-ray diffraction and small-angle X-ray scattering have shown that the water molecules are confined in carbon micropores.29-33 Nevertheless, most studies on the adsorption of water by microporous carbons consider that the surface groups play the main role.7-15,34-42 The focus of many of these studies has been to analyze the role of surface groups (amount and type) by subjecting the ACs to controlled oxidative treatments (in many case very strong, e.g., with hot nitric acid). These treatments can develop a surface chemistry often very different from that which normally prevails on the surface of commercial ACs, leading to higher concentrations of species with different functionalities. Thus, in these studies, the influence of pore size on the mechanism of water adsortion is masked by the higher amount of surface groups. As a consequence, it can be stated that the analysis of water isotherms on porous carbon materials is not sufficiently well understood. In particular, there has been little systematic study of the influence of pore size on the mechanism of water adsorption, and the adsorption of water in the mesopores of AC has scarcely been studied at all. It is noteworthy in this respect that Kaneko recently suggested that water does not adsorb in the mesopores.43,44 In previous studies, we have investigated the water adsorption in AC fibers (ACFs), which are mainly microporous solids with a well-defined porosity and a relatively low surface concentration of oxygenated groups.45 By reducing the influence of the surface complexes, we were able to show that water adsorption in micropores depends on the micropore size, taking place
10.1021/jp010674b CCC: $20.00 © 2001 American Chemical Society Published on Web 07/31/2001
Water Adsorption on Activated Carbons
J. Phys. Chem. B, Vol. 105, No. 33, 2001 7999
TABLE 1: Characteristics of the Activated Carbons (AC) Used sample
KUA1 A SCII (ref. GR 31124A)a BH45 Darko (G-60) BPL (ref. GR 31124E)a Westvaco (SA-30) a
fiber from petroleum pitch fiber from petroleum pitch anthracite phenolic resin coconut
Chemical:KOH Carbonized/N2 -
almond shell bituminous coal
Specially prepared samples.
gradually according to the pore size. First, the narrow micropores and then the wider ones are filled. It was concluded that the adsorbed water in the microporosity is in a solid, ice-like phase, with a density around 0.92 g cm-3. This paper presents the results of an extension of this study to ACs obtained from different precursors, now covering a wide range of pore volumes with materials selected with different contributions from mesoporosity and microporosity to enable the influence of the mesopores on the water adsorption isotherm to be more clearly observed. 2. Experimental Section Water adsorption was studied on a series of commercial activated carbons (BPL, SCII, Darko, and Westvaco) and samples prepared in the laboratory (CFC20, CFS79, KUA1, A, and BH45). Table 1 summarizes the raw materials and activation methods in each case. Activated carbon fibers were prepared by the physical activation of a commercial petroleum pitchbased carbon fiber (Kureka) in CO2 up to a 20% burnoff (CFC20) and in steam up to a 79% burnoff (CFS79);45,46 KUA1 was prepared by chemical activation of a Spanish anthracite47 and BH45 by physical activation of a ligno-cellulose-based carbon,48 while sample A is a phenol-formaldehyde polymer resin char.49 Porous texture analysis of these samples was carried out by gas adsorption (N2 and CO2 at 77 and 273 K respectively, using the Quantachrome Autosorb 6) and by mercury porosimetry (Carlo Erba 2000). The samples were outgassed at 623 K under vacuum, at 10-6 Torr. The Dubinin-Radushkevich (DR) equation7,50 was used to calculate the micropore volume. The different pore volumes used in our discussion were calculated as follows:51 From the CO2 DR plots (relative pressures < 0.015), the volume of narrow micropores (pore size < 0.7 nm) was calculated (VC) . The total micropore volume, Vmic (pore size < 2 nm), was calculated from the N2 DR plot (relative pressures < 0.14) and includes the volume of the narrow micropores and the supermicropores. The mesopore volume, Vmes, (2 nm < pore size < 50 nm) was estimated by combining data from the N2 isotherm (i.e., amount adsorbed between P/P0 ) 0.3-0.7), which gave the volume in pores up to 3 nm radius, with data from mercury porosimetry, which gave the volume in pores from 3 to 25 nm in radius. The macropore volume, Vmac (50 nm < pore size), was obtained from mercury porosimetry. Water adsorption measurements were carried out at 298 K in an automatic volumetric gas adsorption instrument (Belsorp 18). It should be noted that there are difficulties in accurately measuring pressures above 0.98 in more conventional gas
Figure 1. N2 isotherms of the activated carbons.
adsorption equipment, due both to water condensation on the wall of the instrument and to the long time taken to come to equilibrium. This instrument is designed to avoid the condensation of water vapor on the walls of the apparatus and can be operated for long times (40-80 h). Experimental data were corrected for adsorption on the inner wall of the apparatus. A more detailed description of the system is given elsewhere.52 Additionally, a blank run on all the bulbs showed that water adsortion on the inner surface of the glass was negligible. Samples were degassed at 623 K under high vacuum (10-6 Torr). The mechanism of water adsorption was further analyzed by remeasuring the N2 adsorption on ACs with a certain amount of water preadsorbed. To do this, the water adsorption in a sample was stopped at a certain relative pressure; the bulb was closed and then the sample analyzed by N2 adsorption at 77 K. The same procedure was applied to the analysis of the transition between meso- and macroporosity with highly hydrated samples were also analyzed by mercury porosimetry. These highly hidrated samples were immersed in pure distilled water, and after introduced into a desiccator for a period of time. 3. Results and Discussion 3.1. Textural Characterization of Activated Carbons. Figure 1 shows the nitrogen isotherms of the ACs. All samples are microporous and show considerable uptake of nitrogen at low relative pressures ( 0.2 in some samples shows that these are also mesoporous. These isotherms demonstrate that the samples cover a wide range of pore volume, with varying capacity of N2 adsorption. They can be divided into two groups, those which are essentially microporous without any mesoporosity which show true type I isotherms [CFC20, CFS79, SCII, and KUA1] and those which display additional meso- and macroporosity. In the latter group, the volume ratios of each pore type vary significantly. Figure 2 shows the cumulative pore volume distribution obtained from mercury porosimetry. The samples having no macro- and mesoporosity, CFC20, CFS79, and KUA1, are not represented. The results show that SCII has a very small macropore volume, although this is not clearly evident in the N2 isotherm. Samples BH45 and Darko have similar, low mesopore volumes, consistent with the similar shapes of their nitrogen isotherms, but they display quite different macropore volumes. The higher macropore volume of Darko can be partly
8000 J. Phys. Chem. B, Vol. 105, No. 33, 2001
Alcan˜iz-Monge et al.
Figure 2. Cumulative pore volume distributions of the carbons, from mercury porosimetry.
Figure 3. Histograms showing the different pore volumes of the various ACs: narrow microporosity (VC), all microporosity (Vmic), mesoporosity (Vmes), and macroporosity (Vmac).
related to the interparticle space. Sample A contains only mesoporosity but at an appreciable volume. Finally, Westvaco and BPL samples have high mesopore volumes as well as a considerable macropore volume. To analyze the pore volume distribution more completely, Figure 3 shows the volumes of pores in different size ranges. The comparison of both VC (narrow micropore, 0.8), they behave in accord with their different meso- and macropore size distributions. Thus, according to the pore size distribution and the contribution of the different pore volumes, the water isotherm can be type V, with essentially microporous ACs, or type III for ACs, with a wider pore size distribution and similar micro- and mesopore volumes. Thus, the water isotherm on sample A displays a clear distinction between the two regions of pore size, due to it having a well-defined transition between both kinds of porosity. As has been commented previously,45 as the micropore size increases, water adsorption shifts to higher relative pressures. Therefore, when a clear transition does not exist between the micro- and mesoporosity, both the final filling of the micropores and the start of capillary condensation in mesopores can take place in the same range of relative pressures, the overlapping processes giving a single curve. All of these points are reflected in Figure 4b. So it can be seen clearly that two regions of water adsorption take place in the samples BH45Darko, whereas on BPL-Westvaco, the distinction is not so evident. There is a clear correlation with the pore size distributions of the samples (Figure 3). It seems clear from this and the previous study45 that water adsorption up to P/P0 of about 0.8 is due to micropore filling and at higher P/P0 due to the filling of the mesopores and/or macropores. From a visual analysis of all the isotherms in this and the previous work, a value of P/P0 ) 0.82 is a good approximation for the relative pressure at which the micropore volume is filled with adsorbed water for all samples. This approach was used to estimate to the micropore volume. A similar approximation had been made by Lodewyckx and Vansant.54 Table 2 compares the micro and combined meso- and macropore volumes of the samples, estimated from water adsorption, with those from N2 and mercury porosimetry, already discussed. The meso-macropore volumes were calculated from the difference between the amounts of water adsorbed at saturation and at P/P0 ) 0.82. According to the previous work,
Figure 5. Water adsorption isotherms (a) normalized to the value at P/P0 ) 0.82 (N/N0.82); (b) water adsorption isotherms from P/P0 ) 0.82.
we have used the value of 0.92 g cm-3 as the density of water adsorbed in carbon micropores.45 However, water adsorbed in mesopores is likely to have a density closer to that of liquid water, and so, the liquid density value has been used to calculate the volume of pore space filled with adsorbed water at P/P0 > 0.82. Table 2 shows that the micropore volumes obtained from the amount of water adsorbed at P/P0 ) 0.82 agrees quite well with the corresponding N2-derived micropore volumes. The agreement is especially good for the samples with little or no mesoporosity but is remarkable for the others, considering that adsorption in the two types of pores overlaps. This result suggests that the approach is sound and confirms again that water adsorbs in the whole micropore volume. Considering the variety of ACs employed in this study, it seems to be a generalized fact that the water adsorbed in micropores is present in a solidlike structure (density 0.92 g cm-3). This confirms the use of the density of ice to calculate the micropore volume in ACs.45 To analyze more completely the adsorption of water in the micropores, all the samples represented in Figure 4 have been normalized with reference to the value that their presents at P/P0 ) 0.82. Figure 5a shows such normalized plots. From it, we can observe that the isotherm shape is very dependent upon the micropore size distribution of the AC (Figure 3), and it
8002 J. Phys. Chem. B, Vol. 105, No. 33, 2001 further emphasizes the influence exercised by the micropore size in determining the water isotherm shape.34,45,55-57 This is not to deny the importance of surface oxygen complexes, but the water adsorption on these complexes takes place at relative pressures below the steep rise in the isotherm and represents only a small proportion of the total water adsorbed in the micropores,13,54 determining merely the position of the onset of adsorption. A curious general relationship seems to exist (except CFS79 sample) between the slope of the isotherm lineal tract (Figure 5a) and the micropore size distribution. Thus, sample CFC20 has both a high slope of the isotherm lineal tract and a narrow micropore size distribution, whereas sample Westvaco has a minor slope and a broad micropore size distribution (see Figures 3 and 5a). It is also interesting that the isotherms for samples Darko and BH45 (Figure 5a) exhibit two inflections, showing that water adsorption also seems to be quite sensitive to the detail of the micropore size distribution. Table 2 also compares the values of Vmes + Vmac determined from N2 adsorption with the volume occupied by water adsorbed in the region of P/P0 0.82-1, assuming that the latter is in the form of a liquid and hence its density is 1 g cm-3. It appears that the amount of water adsorbed in this range of pore size depends on sample type. Thus, samples BH45 and BPL display similar volumes, indicating that water adsorbs in the whole pore volume, whereas for samples Westvaco and A, this is not always the case. From the values obtained for Darko, BH45, and BPL, it is clear that the water adsorbs in the macropores, since the pore volume obtained from water adsorption is twice as that of the mesopore volume. This is greatly different from that of conventional adsorptives (N2 and C6H6), which do not show adsorption in macropores or in large mesopores.7 This difference is due to the high surface tension of water in comparison with the other liquid adsorptives. Juhola22 suggested that this property of water, together with its small molecule diameter and the fact that it is not strongly adsorbed on activated carbon, makes water a suitable adsorptive for determining the pore size distribution of carbon, allowing it to cover a wider range of pore diameters (2-400 nm) than those of other adsorptives. 22 To more easily compare the isotherms in the range of relative pressure 0.82-1, because there are samples for which the pore volume is not totally filled by the water, they have been normalized using the value at P/P0 ) 0.82 as the origin (Figure 5 b). In general, up to relative pressures of about 0.9-0.95, the order of the isotherms and of the amounts of water adsorbed follows the same trend as that of the mesopore volume (Figure 3). At relative pressures higher than 0.95, there is a sharp increase in the water uptake for BPL and BH45 and also for Darko but with not such a clear discontinuity as that in the latter case. This seems to be indicative of the start of condensation in macropores. The amounts adsorbed at this P/P0 (0.95) are coincident with the mesopore volumes. The concept of capillary condensation would require that the mesopores are filled prior to the macropores, and this is what is observed. A study of the transition in the filling of both types of pore is interesting. For example, BH45 and BPL show a clear transition; for Darko it is more smooth, but for Westvaco and A, it is not evident. For sample A, this is because this material displays very little macroporosity. For BH45 and BPL, the effect is due to the fact that the pore size distribution in the meso/ macropore range is bimodal (Figure 2). Samples Darko and Westvaco have a continuous pore size distribution in this range, which explains why no discontinuity exists in the water isotherm of the former at these high relative pressures. However, the macropore volume of sample Darko is not completely filled
Alcan˜iz-Monge et al. with adorbed water, as shown in Table 2. This is undoubtedly because the macropore volume assessed by mercury penetration includes a significant amount of interparticle pore space in this case. The Westvaco sample should not be expected to show any inflection in the water isotherm at P/P0 > 0.95 because it also has a continuous distribution of pore size. However, it would appear that water adsorption in the mesopores of Westvaco and also of sample A occurs at a P/P0 higher than those of the other samples, and according to Table 2, their meso/ macropore volume is not completely filled. A similar result was obtained with mesoporous carbon aerogels by Hanzawa and Kaneko,43,44 who reported that water does not adsorb in carbon mesopores. However, the above results show that in certain cases, it does. The different behavior of the other two samples is analyzed in the next section. 3.3. Characterization of Porous Texture of Partially Hydrated Samples. To confirm that the mesopore volume of sample A and the meso- and macropore volumes of the Westvaco sample are not completely filled with adsorbed water, the procedure used previously45 to elucidate the mechanism of water adsorption in micropores was adopted, in which samples with water preadsorbed to saturation were further characterized by N2 adsorption. In this procedure, only the Westvaco and sample A showed any N2 adsorption, which demonstrates that there is available surface area in these two samples saturated with water and that the pore space of the other samples is completely filled. Hence, it is clear that there is a meso- and/or macropore volume in which water is not adsorbed in these samples. To study in more detail the mechanism whereby water is adsorbed into the pore structure, a similar procedure was used but with different amounts of preadsorbed water. The water adsorption in a sample was stopped at a certain level of filling. As an example, Figure 6 shows the fractional filling of water used for samples Westvaco and A (Figure 6a,b) and the corresponding N2 isotherms for each (Figure 6 c and d). For a better analysis, Table 3 shows the fractional filling of the different pore volumes with water at each relative pressure of water at which the isotherm was halted. In this procedure, the unfilled micropore volume was estimated at P/P0 ) 0.3 on the nitrogen isotherm of the partially saturated sample (which is very close to the micropore volume) and the unfilled mesopore volume from the difference between this value and the amount adsorbed at P/P0 ) 1. While the estimate of the unfilled micropore volume should be quite accurate, the nitrogen isotherm on these partially saturated materials cannot be used to assess any changes in the macropore volume. As observed, there is a progressive reduction in N2 adsorption capacity with the increase in amount of water preadsorbed, which is similar for all the samples studied. The appreciable N2 adsorption observed in the saturated Westvaco and A samples occurs by capillary condensation in the mesopores and multilayer adsorption on the surfaces of macropores. The above comparison of nitrogen isotherms with the corresponding point on the water isotherm shows that the water adsorbed at low P/P0 produces only a decrease in the micropore volume equivalent to the fractional filling with water (Table 3). Thus, there is a progressive reduction in micropore volume without any change in the mesoporosity until a P/P0 around 0.82, where the micropore volume is nearly filled. This result confirms the approximation made above that in this range of relative pressure, water adsorbs only in micropores. From different experiments, Hanzawa and Kaneko43,44 made a similar conclusion, that the adsorption of water vapor on AC in the
Water Adsorption on Activated Carbons
J. Phys. Chem. B, Vol. 105, No. 33, 2001 8003
Figure 6. Water isotherms on carbons Westvaco (a) and A (b), showing the different degrees of water uptake at which the adsorption was arrested prior to N2 adsorption characterization; the corresponding N2 isotherms of Westvaco (c) and A (d) at the different degrees of water uptake.
TABLE 3: Pore Volume Reduction (%) Due to Different Amounts of Preadsorbed Water, as Deduced from N2 Isotherms sample Westvaco Westvaco Westvaco A A A BPL BPL BH45 darko
P/P0 of preadsorbed water
Vmic (%) precursor
0.60 0.82 1 0.47 0.62 1
22 90 100 70
1 9 73 0
80 100 78 1 100 100
0 65 0 100 100 100
0.79 1 1 1
middle range of P/P0 is not ascribable to a capillary condensation mechanism. It also agrees with the conclusions from a previous study of water adsorption in the micropores of AC fibers45 that narrower micropore are filled first and water is ultimately adsorbed in the whole range of microporosity. The next section will analyze how water adsorbs in the meso- and macropore size range. To investigate more fully the transition from adsorption in mesopores to that in macropores, the characterization of partially
hydrated samples was continued. However, in this case, the analysis of the unfilled pore volume and size distribution must be carried out with mercury porosimetry. In this case, the amount of water adsorbed was expressed as a weight percentage of the AC sample (see Experimental Section). The BPL sample was chosen because it displays a clear transition around P/P0 ) 0.98 in the water isotherm (Figure 5b). Figure 7 shows the cumulative pore volume distribution from mercury porosimetry of this sample degassed and with 130 and 150 wt % of adsorbed water (corresponding to amounts adsorbed at P/P0 > 0.995). The adsorbed water progressively decreases both the meso- and macropore volumes accessible to mercury. In the sample with 150 wt % adsorbed, there is no evidence of mesoporosity and the macropore volume is reduced. Hence, from these experiments, it is evident that water adsorb first in mesopores and then in the macropores. Similar results had been obtained by Lentz and Zhou,58 who concluded that water adsorbs first in the small pores. 3.4. Study of Mechanism of Water Adsorption on AC. The results obtained in this work will now be analyzed in the context of the island cluster and capillary condensation approaches to water adsorption discussed in the Introduction. The results and discussion presented above show that it is reasonable to consider
8004 J. Phys. Chem. B, Vol. 105, No. 33, 2001
Alcan˜iz-Monge et al.
Figure 7. Cumulative pore volume distributions from mercury porosimetry for sample BPL degassed and with 130 and 150 wt % of preadsorbed water.
that water adsorbs principally in the micropores up to about P/P0 ) 0.8, at which point filling of the mesopores begins and then, at P/P0 close to saturation, volume filling of the macropores takes place (Figure 5b). Thus, volume filling of the pores of ACs occurs during water adsorption but via different mechanisms according to the pore size. Considering the two approaches, it is reasonable to conclude that, in principle, both mechanisms are valid but they principally apply to different ranges of relative pressures. Thus, water adsorption at low P/P0 is influenced by the island-cluster mechanism, the micropores are filled with water in an “ice-like” state at P/P0 of about 0.82, and at P/P0 > 0.8, there is capillary condensation. In previous work45 with AC fibers, it was suggested that after the initial clustering process water fills the micropores according to the Polanyi-Dubinin potential theory, or the theory of volume filling of micropores (TVFM).50,59 In this work, we find the same trend in a series of ACs typical of those used in commercial applications (Figure 5a) for the isotherm shape on the range of P/P0 0.3-0.8 depends on the micropore size distribution, in accord with the TVFM theory. This is also in agreement with the conclusion of other researchers that water adsorption on microporous AC with low oxygen contents can be described by the DA approach.54,60 The influence-exercised surface groups is manifested at low relative pressures ( 0.8, the water adsorption is pushed to higher relative pressures as the adsorption temperature is increased. This dependence on temperature is in agreement with the capillary condensation mechanism (see last equation). Hence, these results (Figures 9 and 10), provide further support for the conclusion that the water adsorption at P/P0 > 0.8 is realized according to the capillary condensation mechanism. 4. Conclusions It is shown that the shape of the water isotherm has a clear correlation with the pore size distribution. Thus, water isotherms display type V on essentially microporous ACs, while the presence of meso- and macroporosity gives an isotherm shape
8006 J. Phys. Chem. B, Vol. 105, No. 33, 2001 that tends toward type III. Thus, water adsorption is a good technique to assess all ranges of pore size, at least semiquantitatively. The slope of the isotherm lineal tract (on the range P/P0 ) 0.3-0.8) is related to the micropore size distribution. The presence of surface groups affects the isotherm in two ways; they control the relative pressure at the onset of adsorption in micropores and the filling of meso- and macropores by capillary condensation through their effect on the contact angle with liquid adsorptive prevailing at the pore wall. However, unless there is a pore-blocking effect, they do not influence the extent of volume filling of micropores, which takes place via a volume filling mechanism. The density of the adsorbed phase in micropores is close to that of ice and probably close to the liquid value in meso- and macropores. Micropore filling is not complete until a P/P0 of about 0.82, when capillary condensation begins in samples with relatively low surface polarity. Condensation in macropores can be observed with this adsorptive, but only at relative pressures greater than 0.95. This is contrast to the limitation in pore size that can be assessed by the conventional adsorptive, nitrogen. Acknowledgment. J. Alcan˜iz would like to thank The Leverhulme Trust for the award of a visiting fellowship to the Department of Materials at the University of Leeds, U.K., where part of this collaborative study was carried out. We also wish to thank Project MEC-CICYT (Proyect No. PB98-0983). References and Notes (1) Bansal, R. Ch.; Donnet, J.; Stoeckli, F. ActiVe Carbon; Marcel Dekker: New York, 1988. (2) Lowell, S.; Shields, J. E. Powder, Surface Area and Porosity, 3rd ed.; Chapman and Hall: Bristol, 1991., (3) Jankowska, H.; Swiatkowski, A.; Choma, J. In ActiVe Carbon; Kemp, T. J., Ed.; Ellis Horwood: Chischester, 1991. (4) Suzuki, M.; Doi, H. Carbon 1982, 20, 441. (5) Barton, S. S.; Koresh, J. E. Carbon 1984, 22, 481. (6) O’Koye, I. P.; Benham, M.; Thomas, K. M. Langmuir 1997, 13, 4054. (7) Gregg, S. J.; Sing, S. K. W. Adsorption, Surface Area and Porosity, 2nd ed.; Academic Press: London, 1982. (8) Dubinin, M. M. Carbon 1980, 18, 355. (9) Walker, P. L. Jnr.; Janov, J. J. Colloid Interface Sci 1968, 28, 499. (10) Barton, S. S.; Koresh, J. E. J. Chem. Soc., Faraday Trans. 1 1983, 79, 1147, 1157, 1165. (11) Kaneko, K.; Inouke, K. Carbon 1986, 8, 772. (12) Carrott, P. J. M.; Kenny, M. B.; Roberts, R. A.; Sing, K. S. W.; Theocharis, C. In Characterisation of Porous solids II; Rodriguez-Reinoso, F., Rouquerol, J., Sing, K. S. W., Unger, K. K, Eds.; Elsevier: Amsterdam, 1991; p 685. (13) Rodriguez-Reinoso, F.; Molina-Sabio, M.; Mun˜ecas, M. A. J. Phys. Chem. 1992, 96, 2707. (14) Bradley, R. H.; Rand, B. J. Colloid Interface Sci. 1995, 169, 168. (15) Vartapetyan, R. Sh.; Voloshchuk, A. M. Russ. Chem. ReV. 1995, 64, 985. (16) McBain, J. W.; Porter, J. L.; Sessions, R. F. J. Am. Chem. Soc. 1933, 55 (5), 2294. (17) Juhola, A. J.; Wiig, E. O. J. Am. Chem. Soc. 1949, 71, 2069. (18) McDermott, H. L.; Arnell, J. C. J. Phys. Chem. 1954, 58, 492. (19) Kadlec, O.; Varhanikova, A.; Zukal, A. Carbon 1970, 8, 321. (20) Bansal, R. C.; Dhami, T. L.; Parkash, S. Carbon 1978, 16, 389. (21) Mahle, J. J.; Friday, D. K. Carbon 1989, 27, 835. (22) Juhola, A. J. Kem. - Kemi 1977, 4, 543. (23) Sutherland, J. W. In Porous Carbon Solid; Bond, R. L., Ed.; Academic Press: London, 1970; pp 1-64.
Alcan˜iz-Monge et al. (24) Pierce, C.; Smith, R. N. J. Phys. Chem. 1950, 54, 784. (25) Dubinin, M. M.; Zaverina, E. D.; Serpinsky, V. V. J. Chem. Soc. 1955, 1760. (26) Dubinin, M. M.; Sherpinsky, V. V. Carbon 1981, 19, 402. (27) Mu¨ller, E. A.; Gubbins, K. E. Carbon 1998, 36, 1433. (28) McCallum, C. L.; Bandosz, T. J.; McGrother, S. C.; Mu¨ller, E. A.; Gubbins, K. E. Langmuir 1999, 15, 533. (29) Iiyama, T.; Nishikawa, K.; Suzuki, T.; Otowa, T.; Hijiriyama, M.; Nojima, Y.; Kaneko, K. J. Phys. Chem. B 1997, 101, 3037. (30) Iiyama, T.; Nishikawa, K.; Suzuki, T.; Kaneko, K. Chem. Phys. Lett. 1997, 274, 152. (31) Iiyama, T.; Nishikawa, K.; Otowa, T.; Suzuki, T.; Kaneko, K. In Characterisation of Porous Solids IV.; McEnaney, B., May, T. J., Rouquerol, J., Rodriguez-Reinoso, F., Sing, K. S. W., Unger, K. K. K., Eds.; Royal Society of Chemistry: London, 1998; 41. (32) Iiyama, T.; Ruike, M.; Suzuki, T.; Kaneko, K. In Characterisation of Porous Solids V.; Unger, K. K. K., Kreysa, G., Baselt, J. P., Eds.; Elsevier Science: Amsterdan, 2000; p 355. (33) Kaneko, K. K. Carbon 2000, 38, 287. (34) Salame, I. I.; Bandosz, T. J. Colloid Interface Sci. 1999, 210, 367. (35) Salame, I. I.; Bandosz, T. Langmuir 1999, 15, 587. (36) Kaneko, K.; Katori, T.; Shimizu, K.; Shindo, N.; Maeda, T. J. Chem. Soc., Faraday Trans. 1992, 88, 1305. (37) Kaneko, Y.; Ohbu, K.; Uekawa, N.; Fujie, K.; Kaneko, K. Langmuir 1995, 11, 708. (38) Stoeckli, F.; Kraehenbuehl, K.; Morel, D. Carbon 1983, 21, 589. (39) Carrasco-Marı´n, F.; Mueden, A.; Centeno, T. A.; Stoeckli, F.; Moreno-Castilla, C. J. Chem. Soc., Faraday Trans. 1997, 93, 2211. (40) Wintgens, D.; Lavanchy, A.; Stoceckli, F. Ads. Sci. Technol. 1999, 17, 761. (41) Stoeckli, F.; Lavanchy, A. Carbon 2000, 38, 475. (42) Lo´pez-Ramo´n, M. V.; Stoeckli, F.; Moreno-Castilla, C.; CarrascoMarı´n, F. Carbon 2000, 38, 825. (43) Hanzawa, Y.; Kaneko, K. Langmuir 1997, 13, 5802. (44) Kaneko, K.; Hanzawa, Y.; Iiyama, T.; Kanda, T.; Suzuki, T. Adsorption 1999, 5, 7. (45) Alcan˜iz-Monge, J.; Linares-Solano, A.; Rand, B. J. Phy. Chem. B 2000, submitted for publication. (46) Alcan˜iz-Monge, J.; Cazorla-Amoro´s, D.; Linares-Solano, A. Carbon 1997, 35, 1665. (47) Illa´n-Go´mez, M. J.; Garcı´a-Garcı´a, A.; Salinas-Martı´nez de Lecea, C.; Linares-Solano, A. Energy Fuels 1996, 10, 1108. (48) Cazorla-Amoro´s, D.; Ribes-Pe´rez, D.; Roma´n-Martı´nez, M. C.; Linares-Solano, A. Carbon 1996, 34, 869. (49) Roma´n-Martı´nez, M. C.; Cazorla-Amoro´s, D.; Linares-Solano, A.; Salinas-Martı´nez de Lecea, C.; Atamny, F. Carbon 1996, 34, 719. (50) Dubinin, M. M.; Raduskevich, L. V. Proc. Acad. Sci. SSSR 1947, 55, 331. (51) Rodrı´guez-Reinoso, F.; Linares-Solano, A. In Chemistry and Physics of Carbon; Thorwer, H., Ed.; Marcell Dekker Inc: New York, 1988; pp 2-146. (52) Naono, H.; Hakuman, M. J. Colloid Interface. Sci. 1991, 145, 405. (53) Sing, K. S. W.; Everett, D. H.; Haul, R. A. W.; Moscou, L.; Pierotti, R. A.; Rouquerol, J.; Siemieniewska, T. Pure Appl. Chem. 1985, 57, 603. (54) Lodewyckx, P.; Vansant, E. F. Carbon 1999, 37, 1647. (55) Tsunoda, R. J. Coll. Int. Sci. 1990, 137, 563. (56) Carrott, P. J. M. Carbon 1991, 29, 507. (57) Freeman, J. J.; Tomlinson, J. B.; Sing, K. S. W.; Theocharis, C. R. Carbon 1993, 31, 865. (58) Lentz, H.; Zhou, Y. In Characterisation of Porous solids II; Rodriguez-Reinoso, F., Rouquerol, J., Sing, K. S. W., Unger, K. K, Eds.; Elsevier: Amsterdam, 1991; p 499. (59) Dubinin, M. M. Chem. ReV. 1960, 60, 235. (60) Stoeckli, F.; Jakubov, T. S.; Lavanchy, A. J. Chem. Soc., Faraday Trans. 1994, 90, 783. (61) Naono, H.; Shimoda, M.; Morita, N.; Hakuman, M.; Nakai, K.; Kondo, S. Langmuir 1997, 13, 1297. (62) Hassan, N. M.; Ghosh, T. K.; Hines, A. L.; Loyalka, S. K. Carbon 1991, 29, 681. (63) Do, D. D.; Do, H. D. Carbon 2000, 38, 767. (64) Adamson, A. W. Physical Chemistry of Surfaces, 5th ed.; Wiley: New York, 1990; p 397.